of implantable glucose biosensors
1Biomedical Engineering Theme, Institute for Environment, Health and Societies, Brunel University London, Uxbridge UB8 3PH, United Kingdom
2Department of Mechanical, Aerospace and Civil Engineering, College of Engineering, Design and Physical Sciences, Brunel University London, Uxbridge UB8 3PH, United Kingdom
3UCL Centre for Nanotechnology and Regenerative Medicine, Division of Surgery and Interventional Science, University College London, London NW3 2PF, United Kingdom
Received 16 July 2017; revised 13 October 2017; accepted 5 December 2017
Published online 23 December 2017 in Wiley Online Library (wileyonlinelibrary.com). DOI: 10.1002/jbm.a.36308
Abstract: In vivotissue responses and functional efficacy of electrospun membranes based on polyurethane (PU) and gela- tin (GE) as biomimetic coatings for implantable glucose bio- sensors was investigated in a rat subcutaneous implantation model. Three electrospun membranes with optimized fiber diameters, pore sizes, and permeability, both single PU and coaxial PU-GE fibers and a solvent cast PU film were implanted in rats to evaluate tissue responses. For functional efficacy test- ing, four sensor variants coated with the above mentioned electrospun membranes as mass-transport limiting and outer- most biomimetic coatings were implanted in rats. The electro- spun PU membranes had micron sized pores that were not permeable to host cells when implanted in the body. However, PU-GE coaxial fiber membranes, having similar sized pores, were infiltrated with fibroblasts that deposited collagen in the membrane’s pores. Such tissue response prevented the
formation of dense fibrous capsule around the sensor coated with the PU-GE coaxial fiber membranes, which helped improve thein vivosensitivity for at least 3 weeks compared to the traditional sensors in rat subcutaneous tissue. Further- more, the betterin vitrosensor’s sensitivity due to electrospun PU as the mass-transport limiting membrane translated to bet- terin vivosensitivity. Thus, this study showed that electrospun membranes can play an important role in realizing longin vivo sensing lifetime of implantable glucose biosensors.VC2017 The Authors Journal of Biomedical Materials Research Part A Published by Wiley Periodicals, Inc. J Biomed Mater Res Part A: 106A: 1072–1081, 2018.
Key Words: continuous glucose monitoring, electrospun coaxial fiber membranes, implantable electrochemical sensor, in vivofunctional efficacy, tissue reactions
How to cite this article: Burugapalli K, Wijesuriya S, Wang N, Song W. 2018. Biomimetic electrospun coatings increase the in vivosensitivity of implantable glucose biosensors. J Biomed Mater Res Part A 2018:106A:1072–1081.
Dynamic foreign body reactions on the sensor surface have been the crucial barrier for the design of reliable, long-term implantable glucose biosensors.1–5
Speciﬁcally, biofouling, inﬂammation, ﬁbrosis, receding microvasculature, and extracellular release of lysosomal contents are responsible for the unpredictable negative drift in sensor signal.1
How- ever, from a practical perspective, three main aspects affect the implanted glucose biosensor function: (1) robustness of sensor design, (2) biofouling by proteins and cells, and (3) ﬂuctuation of interstitial ﬂuid levels at implant site.1
Electrochemical glucose biosensors are known to lose sensitivity as soon as they are implanted followed by a downward drift until failure. From the sensor design per- spective, Valdes and Moussy showed that the activity of the immobilized glucose oxidase (GOD) enzyme is a fundamen- tal limiting factorin vivo, as it deteriorates due to
accumulation of H2
in the sensor element.6
Moussy et al.
developed a sensor design with a coil reinforced with cotton that allows loading of excess enzyme as working electrode to cope with the demands for long-term implantation.7–12
This sensor design provides sensitivities>40 nA/mM,10
which are much better compared to sensors tested earlier, because current measurements in pA/mM are susceptible to large ﬂuctuationsin vivo.5,13,14
Biofouling signiﬁcantly lowers the sensitivity of implanted sensors and its effect at least initially can be minimized by tailoring surface chemistry of the sen- sors.1–4,15
However, it cannot stop the eventual adhesion and spreading of macrophages and foreign body giant cells on sensor surface that signiﬁcantly reduce the quantity of glucose reaching the sensor.5
The tissue microenvironment inherently has much lower (interstitial) ﬂuid levels compared toin vitro
Correspondence to: K. Burugapalli; e-mail: firstname.lastname@example.org
Contract grant sponsor: Royal Society, UK; contract grant number: RG2010R1 - RG100129
Contract grant sponsor: National Institute of Health, USA; contract grant number: 7R01EB001640-05
This is an open access article under the terms of the Creative Commons Attribution-NonCommercial License, which permits use, distribution and reproduction in any
simulated body (100%) ﬂuids.16–18
Further, the interstitial ﬂuid levels at the implant site vary signiﬁcantly depending on the stage of inﬂammation and mechanical disturban- ces.1–4
Helton et al. also reiterate the role of mechanical (compressive, tensile, shear and contractile) forces and micromotion (due to breathing, and pulsing blood vessels), which chronically disrupt the tissue stabilization during the natural wound healing process causing unpredictable ﬂuctu- ations in interstitial ﬂuid levels resulting in erratic sensor signals.1
Biomaterial coatings can provide the required chemical, structural and mechanical buffer zone for fulﬁlling the ulti- mate goal of long-term implantable glucose biosen- sors.5,14,19–21
Earlier, we reported electrospun membranes based on polyurethane (PU) and gelatin (GE) both in single polymer and coaxial dual polymer formats to coat miniature glucose biosensors, and systematically characterized their physical, chemical and mechanical properties, as well as their effect on sensor sensitivity.10–12
The ﬁbroporous mem- branes, due to their high pore volume, helped us achieve signiﬁcantly higher preimplantation sensor sensitivity com- pared to the traditional solvent-cast epoxy-PU (EPU) mem- branes.10,12
Here, we investigate if the higherin vitro
sensitivity translates to thatin vivo. Furthermore, Sanders
et al. showed that ﬁber diameters of 1 to 5.9lm prevent
ﬁbrous capsule formation around electrospun membranes.22
Hence, we envisaged biomimetic 6PU10GE coaxial ﬁber membranes would prevent not only the ﬁbrous capsule for- mation, but also the barrier cell layer formation at the sen- sor–tissue interface.
Current study evaluated the tissue responses to four implant variants: three electrospun membranes namely, 8PU, 12PU, and 6PU10GE (wherein the number preﬁx indi- cates the concentration [wt %] of the polymer solution used to electrospin), and one solvent cast nonporous PU-ﬁlm (control). Thein vivo
functional efﬁcacy of electrospun membranes in mass transport limiting (8PU) and tissue engineering (12PU and 6PU10GE) roles on the surface of implantable glucose biosensors was also assessed. Signiﬁ- cant ﬁndings were that betterin vitro
sensitivity of sensors having electrospun membrane for mass transport-limiting translated to betterin vivo
sensitivity, and the biomimetic 6PU10GE coatings prevented ﬁbrous capsule formation on sensor surface, thus improving sensor sensitivity for at least 3 weeks.
MATERIALS AND METHODS
Thermoplastic PU (SelectophoreTM
), GE from porcine skin (type A), tetrahydrofuran (THF),N,N-dimethylformamide
(DMF), bovine serum albumin (BSA), glutaraldehyde (GA) grade I, 50% and grade II, 25%, GOD (EC 126.96.36.199, Type X- S,Aspergillus niger, 157 500 U/g; Sigma), ATACS 5104/
4013 epoxy adhesive, Brij 30, D-(1)-glucose, hydrochloric acid, nitric acid, ammonium hydroxide, neutral buffered formalin (4%), Mayer’s hematoxylin, Eosin Y, Masson’s Tri- chrome kit, xylene, and 0.01M
phosphate buffered saline (PBS) pH 7.4 tablets were purchased from Sigma-Aldrich
(UK). Glacial acetic acid, absolute ethanol, 2,2,2-triﬂuoroe- thanol (TFE), and basic histology consumables were pur- chased from Fisher (UK). Teﬂon-coated platinum–iridium (Pt/Ir) (9:1 in weight, Ø 0.125 mm) and silver wires (Ø 0.125 mm) were obtained from World Precision Instruments (Sarasota, FL). Sprague Dawley rats (Harlan UK, Oxon, UK) weighing between 175 and 200 g were housed in the experimental animal facility at Brunel Uni- versity. All animal procedures had ethical approval from the ‘Animal Welfare Ethical Review Board’ of Brunel Uni- versity and covered under the appropriate project (PPL No. 70–6993) and personal (PIL No. 70–21528) licenses from Home Ofﬁce, UK. Home ofﬁce, UK guidelines for the care and use of laboratory animals (Animals [Scientiﬁc Procedures] Act 1986) were observed. Isoﬂuorane (ISO- FloVR
), ketamine hydrochloride (Ketaset), xylazine (Chana- zine), buprenorphine hydrochloride (Vetergesic), soft parafﬁn (Lacri-lube), atipamezole hydrochloride (ATIPAM), sodium pentobarbitone (Euthatal), and carprofen (RIMADYL) were supplied by Lab Services (London, UK).
5–0 Polygalactin and Prolene (Johnson & John- son) sutures were purchased from Vet Tech Solutions (Cheshire, UK). Surgical consumables were purchased from Barrier Healthcare (Lincolnshire, UK). ALPHELYS RCL-2 formalin-free ﬁxative was purchased from Mitogen (UK). Abbott FreeStyle Lite blood glucose meter and test strips were purchased from Point Pharmacy (UK). Medical oxygen cylinders were supplied by Air Liquide UK. Deion- ized water puriﬁed using a Barnstead water puriﬁcation system was used for all experiments.
Electrospinning single and coaxial ﬁber membranes
The methods for traditional and coaxial electrospinning of PU and PU-GE (coaxial) ﬁber membranes both on static plate collector and directly on the miniature sensor surface using a dynamic collector were presented in our earlier reports.10–12
The materials and parameters for electrospin- ning are summarized in Table I.
Sensor preparation and designations
The method for sensor manufacture was described in our previous reports, except that the Pt-Ir working electrode coil in this study had an additional interference reducing layer.10,23
The bare cotton-reinforced Pt-Ir coil was coated with a polyphenylenediamine layer by electropolymeriza- tion at 0.7V versus standard calomel electrode in a PBS containing 5 mM phenylenediamine, 20 U/mL GOD, and 1lL/mL 0.25% GA.7,10,23
Figure 1 shows the schematic representation of the sensor design and function as well as the scanning electron microscopy (SEM) images show- ing the cross-section of the sensors tested in this study.
The typical working electrode had a cotton reinforced Pt/
Ir coil (designated as Pt) coated with GOD immobilized
on BSA using GA crosslinking. The base Pt-GOD sensors
were coated with either EPU or electrospun 8PU mem-
branes. The respective sensors were designated as Pt-
GOD-EPU and Pt-GOD-8PU. To test the efﬁcacy ofORIGINAL ARTICLE
electrospun membranes as tissue engineering sensor sur- face coatings, two membrane conﬁgurations, namely, 12PU and 6PU10GE were used. The four sensor conﬁgurations
tested forin vivo
functional efﬁcacy were Pt-GOD-EPU, Pt- GOD-8PU-12PU, Pt-GOD-EPU-12PU, and Pt-GOD-EPU- 6PU10GE (Table I).
Test Implant Designation
Electrospinning Parametersa Collector; Flat-Tip
Spinneret Solution Parameters
Physical Parameters (Voltage;
Flow Rate; Distance) Biocompatibility testing (131 cm2sheets)
PU film n/a n/a n/a
8PU Static; 22G needle 8% PU in 40:60 w/w THF:DMF 21 kV; 0.6 mL/h; 22 cm
12PU Static; 22G needle 12% PU in 50:50 w/w THF:DMF 20 kV; 1.2 mL/h; 22 cm
6PU10GE Static;21G core/10G
shell coaxial needle
6% PU in TFE (core) and 10%
GE in TFE (shell)
13.25 kV; 0.8 mL/h (core) and 1.2 mL/h shell; 15 cm In vivofunctional efficacy testing of implantable continuous glucose monitoring sensors
Pt-GOD-EPU n/a n/a n/a
Pt-GOD-8PU-12PU Dynamic; 22G needle 8% PU in 40:60 w/w THF:DMF followed by 12% PU in 50:50 w/w THF:DMF
21 kV; 0.6 mL/h; 22 cm fol- lowed by 20 kV; 1.2 mL/h;
Pt-GOD-EPU-12PU Dynamic; 22G needle 8% PU in 50:50 w/w THF:DMF 20 kV; 1.2 mL/h; 22 cm Pt-GOD-EPU-6PU10GE Dynamic;21G core/10G
shell coaxial needle
6% PU in TFE (core) and 10%
GE in TFE (shell)
13.25 kV; 0.8 mL/h (core) and 1.2 mL/h shell; 15 cm
aAmbient temperature and humidity for all electrospinning was 20628C and 4065%, respectively.
FIGURE 1. The design of the amperometric sensor used in this study. (a) A schematic representation of the sensor design and function; inset—
light microscopy photo to illustrate the size of the working electrode, (b, c) scanning electron microscopy images showing the cross-section of the sensors, wherein 1 is cotton, 2 is Pt-Ir coil, 3 is GOD immobilized on BSA using GA crosslinking, 4 is EPU mass transport limiting mem- brane, 5 is electrospun membrane as tissue engineering coating, and 6 is electrospun membrane as mass transport limiting membrane, (c) inset—SEM image showing surface porosity of electrospun coating on sensor.
Crosslinking of GE
The GE in the 6PU10GE coaxial ﬁbers of the electrospun sheets or coatings on sensors was stabilized by GA cross- linking in a GA vapor environment in a vacuum desiccator with the desiccant replaced by 10 mL of 25% aqueous GA solution for three days.
Sensor calibration and testing
Preimplantation sensitivity of the test sensors was meas- ured using Apollo 4000 Analyser (World Precision Instru- ments, Sarasota, FL).10
Sensors were equilibrated in PBS at an applied voltage of 0.7V between the Pt-Ir working elec- trode and the Ag/AgCl reference electrode, while continu- ously stirring the PBS solution. Calibration plots for the sensors were obtained by measuring current while increas- ing the glucose concentration (0–30 mM). The sensitivity (S) of each sensor was calculated using the equation:
mM are the steady state currents for 15 and 5 mM glucose concentration, respectively.
Tissue response evaluation
The tissue responses to the test membranes (13
sheets) were evaluated using male Sprague Dawley rats acclimatized to local environment for 1 week prior to sur- gery. The rats were anaesthetized with ketamine (80 mg/kg) and xylazine (10 mg/kg) and eyes lubricated with Lacri-lube.
Subcutaneous injections of 0.05 mg/kg buprenorphine hydrochloride and 10 mg/kg carprofen were used as analge- sics. The dorsal skin was shaved and disinfected with iodine.
Along the dorsal midline, three 1.5 cm longitudinal incisions were made, about 3 cm apart. At each incision, two lateral subcutaneous pockets were made. In each pocket one test membrane was inserted at the subcutaneous level about 1 cm away from the incision. Prior to implantation, the differ- ent scaffolds were sterilized by their incubation in 70% etha- nol for 1 h followed by washing in several changes of sterile saline. The incisions were closed using a degradable Ethi- conTM
5–0 Polygalactin. Following implantation, atipamezole hydrochloride was administered for reversal of the sedative effects of xylazine. The rats were given standard pellet diet and fresh water. The implant sites were physically observed at regular intervals. A total of six rats were divided into two groups of three each. Four implant variables: PU ﬁlm, 8PU, 12PU, 6PU10GE were assessed in this study. Per time point, three samples of each implant variable were implanted. The two groups of rats were sacriﬁced after 4 and 9 weeks, respectively, and subsequently the implant sites were har- vested and ﬁxed in RCL-2 formalin free ﬁxative.
RCL-2 ﬁxed tissues were dehydrated through graded ethyl alcohol solutions (70, 95, and 100%), cleared with xylene and embedded in parafﬁn. Seven-micrometer thick parafﬁn sections were stained with hematoxylin and eosin (H&E), and Masson’s trichrome (MT). The stained sections were
observed under light microscope and digital images were captured using SP-500 POL microscope equipped with Mini- cam DCM 1.3M USB 2.0 digital camera (Brunel Microscopes, Bristol, UK).
Subcutaneous implantation of glucose sensors
Sensor conﬁgurations Pt-GOD-8PU-12PU, Pt-GOD-EPU-12PU, Pt-GOD-EPU-6PU10GE, and Pt-GOD-EPU (n5
6 for each con- ﬁguration) were implanted in 12 rats. The method was simi- lar to that described above for implantation of membranes in subcutaneous tissue. However, each rat received two sensors and the incisions were done perpendicular to the axis of dor- sal midline over the shoulder blade. In each pocket, the sen- sor was inserted parallel to the dorsal midline and the sensing electrodes away from the neck and the leads exiting skin close to the neck. For implantation, the sensors were reinforced with silicon tubing (U1/16’) leaving electrodes and leads at either end uncovered. A knot was then made in the middle section covered with silicone tubing and either ends of the silicon tubing sealed using epoxy resin (ATACS).
During implantation, the knot was threaded with a nonde- gradable EthiconTM
suture and immobilized in the subcutaneous tissue, such that the leads exited to exterior at the incision in the skin. The incision in the skin was then closed using a degradable Ethicon 5–0 Polygalactin.
In vivofunctional efﬁcacy testing of glucose sensors
Sensor testing was performed at 1, 3 and 9 weeks after implantation on each rat. Anesthesia was induced and main- tained either by intraperitoneal (IP) injection of sodium pentobarbitone or by inhalation of isoﬂurane to test the effect of anesthesia on blood glucose levels. With pentobar- bitone, anesthesia was induced by IP injection of 0.2 mL of 50 mg/mL pentobarbitone and then maintained by a further 3 to 4 injections of 0.1 mL 50 mg/mL pentobarbitone at approximately, 20, 50, 80, 140 min, and 0.5 to 1 L/min oxy- gen supplied continuously through a mask. With isoﬂurane, anesthesia was induced ﬁrst by placing the rat in a plexi- glass chamber and ﬂowing isoﬂurane and oxygen at 2.5%
and 1 L/min, respectively, through the chamber and then transferring the anesthetized rat on to a heated mat, a mask ﬁtted and ﬂowing1% isoﬂurane and 0.5 to 1 L/min oxy-
gen to maintain anesthesia for the duration of the testing.
Buprenorphine hydrochloride and carprofen were adminis- tered for analgesia. Within 15 to 20 min of induction of anesthesia, the sensors were connected to the Apollo 4000 Analyzer to log the change in current as a function glucose concentration at an applied potential of 0.7V. Once the base- line current was established, an IP injection of 0.7 mL of 50% glucose in saline (1 mg/kg). Blood glucose concen- tration were also measured at5 min intervals using a
commercial glucose monitor—Freestyle Lite by withdrawing blood drops from an incision made at the tip of rat’s tail.
The tests typically took 2 h and 196
16 min. Thein vivo
sensitivity of the sensors was calculated using the equation:
is the difference of current between the peak and the baseline, andDC
the corresponding difference in con- centration of blood glucose as measured with commercial glucometer. Following the third functional efﬁcacy test at 9 weeks after implantation, the rats were euthanized with a 1 mL IP injection of 200 mg/mL pentobarbitone. The sensor implant sites were harvested, ﬁxed in RCL-2 ﬁxative, and processed for histopathology.
Statistical analyses were carried out using IBM SPSS (v.20) statistical software. Statistical variances between groups were determined by analysis of variance. Tukey’s test was used forpost hoc
evaluation of differences between groups.
0.05 was considered statistically signiﬁcant. All data is presented as mean6
standard error of mean.
RESULTS AND DISCUSSION
Reproducible production of transmembrane interconnectiv- ity of pores, high pore volumes and uniform thickness proved useful with electrospun PU as mass-transport limit- ing membranes for glucose biosensors.10,11
Electrospun membranes are also widely researched and utilized as tis- sue engineering scaffolds.24
In this study, we investigated the role of electrospun membranes as both mass-transport limiting and tissue engineering coatings to prolong thein vivo
sensing lifetime of implantable glucose biosensors.
The properties of the membranes tested in this work are summarized in Table II.10–12
8PU, 12PU, and 6PU10GE membranes had average ﬁber diameters and average pore sizes of 0.347, 1.102, and 1.15mm, and 0.8, 1.06, and 1.54 mm, respectively. Further, the membranes had average elas-
tic moduli of 2300, 970, and 930 kPa, respectively, which are higher compared to the 2.75 to 240 kPa range reported for rat subcutaneous and skin tissue.25
Tissue reactions to electrospun membranes implanted in subcutaneous tissue
Following surgery, all rats recovered normally and survived the duration of the experiments. The incision and implant sites did not show any ulceration, pus, discharge or infection. No obvious swelling of the implants sites was visible.
Histologically, all the scaffolds were intact until the end of study at 9 weeks. Figure 2(a,b) show the histology of subcutaneous tissue structure on the nonporous
8PU 12PU 6PU10GE PU Filma
Fiber diameter (mm) 0.34760.087 1.10260.210 1.1560.13 -
Thickness (mm) 23.564.8 133.0628.3 44.562.2 71.6616.8
Pore volume (%) 44.1962.54 65.4061.85 63.3361.34 -
Pore size (mm) 0.80 1.06 1.54 -
Contact angle 104.38 122.58 08 868
Young’s Modulus (MPa) 2.360.85 0.9760.049 0.9360.14 2.860.43
UTS (MPa) 5.862.13 3.160.06 1.8360.22 8.162.00
Strain at break (%) 191.2661.10 261.0612.09 133.2967.17 849.76258.8
aNonporous solvent cast PU film was used as the control.
FIGURE 2. Light microscopy images showing H&E stained subcutane- ous tissue above the PU film implant following 4 weeks of implanta- tion (a) and its magnified section (b) and 9 (c), where M is subcutaneous smooth muscle, NF is native fibrous tissue, F is fibrous tissue (capsule) surrounding the implant I.
PU ﬁlm implant (I) surface at 4 weeks after implantation.
About three cell-layers’ thick ﬁbrous capsule (F) was observed on the implant surface. Between the dense ﬁbrous tissue and the subcutaneous smooth muscle (M) layers was a thick layer of typical subcutaneous native ﬁbrous (NF) tis- sue. Several blood capillaries/vessels were also seen at the interface between the NF tissue and the dense ﬁbrous tissue surrounding the implant. At 9 weeks [Fig. 2(c)], the ﬁbrous capsule became thicker (100mm). The cells in the ﬁbrous
tissue were primarily ﬁbroblasts (spindle shaped cells each with a oval shaped active nucleus) at 4 weeks, while at 9 weeks majority of the ﬁbroblasts changed into ﬁbrocytes (inactive ﬁbroblasts, containing thin and long nucleus hav- ing inactive condensed genetic material).26
No immune cells were observed in the ﬁbrous tissue surrounding the PU ﬁlms, indicating the inert nature of the PU material.
Electrospinning introduced ﬁbro-porous structures in 8PU and 12PU membranes. However, when they were implanted in the body, their pore sizes were too small (1lm) to allow inﬁltration of cells into the bulk of the
membranes. Hence, the tissue responses to both 8PU and 12PU were like that observed for nonporous PU ﬁlm at both time points (Fig. 3). The small pore sizes can be attrib- uted to the nature of deposition of ﬁbers by electrospinning.
The ﬁbers fuse at contact points with neighboring ﬁbers resulting in a rigid ﬁbrous mesh.27,28
However, 6PU10GE coaxial ﬁber membranes, having simi- lar pore size (1.5mm), allowed host cell inﬁltration into its
ﬁbro-porous bulk (Fig. 4). The immediate surface of the host cell inﬁltrated 6PU10GE membrane, unlike that of 8PU and 12PU, was not covered by dense ﬁbrous encapsulation. But, the cell content in this layer was signiﬁcantly higher, with pri- marily macrophages indicating an active resorption of GE [Fig. 4(a–d)]. Some lymphocytes were also observed
indicating a mild immune response to GE, which could further accelerate resorption of GE. The blue staining in the MT stained histology sections is collagen. At 4 weeks, hardly any blue staining was seen within the 6PU10GE membrane [Fig.
4(b)]. But by 9 weeks, collagen deposition was seen within the 6PU10GE implant matrix [Fig. 4(d)]. GE, being an extrac- ellular matrix (ECM) derivative, is susceptible to enzymatic degradation, and its resorption would make the thin PU cores discreet and ﬂexible allowing movement of cells within the scaffold. The tiny darkly stained structures within the scaffold indicate cells attached to the individual electrospun ﬁbers along the ﬁber axis [Fig. 4(a,c)]. Such cell adhesion to ﬁbers also indicates that the cells are ﬁbroblasts. Occasional pres- ence of larger cells within the scaffold was also indicative of inﬁltration of larger cells (10mm) through displacement of
ﬂexible ﬁbers. This result demonstrates that the rigidity due to fusion of neighboring ﬁbers can be overcome by using a degradable coating on the electrospun ﬁber surface [Fig. 4(a–
d)]. Zhang et al. also reported partial cellular inﬁltration into electrospun membranes having ﬁber size around 1lm in an in vitro
cell culture study for composite ﬁbers that were elec- trospun with blended solutions of polycaprolactone and GE.29 In vivofunctional efﬁcacy testing
Following surgery for implantation of sensors, all rats recov- ered normally and survived the duration of the experiments (9 weeks) without any adverse events at the implants sites.
The rats weighed 2576
18 g at the time of sensor implanta- tion, and gained weight consistently, with average weights of 2966
24 and 3786
30 g at 1, 3 and 9 weeks, respectively.
Effect of anesthesia on blood glucose levels.
Glucose toler- ance test provides a means to verify the functional efﬁcacy
FIGURE 3. Light microscopy images showing the tissue-implant interface for: (a, b) 8PU and (c, d) 12PU; at (a, c) 4 weeks and (b, d) 9 weeks of implantation; (a, d) [MT stained and (b, c)] H&E stained sections, where A is subcutaneous fat (adipose), F is fibrous tissue (capsule) surround- ing the implant I.
of sensors implanted for continuous glucose monitoring.
However, such testing, in the absence of wireless means of logging the sensor output, requires the use of general anes- thesia. Anesthetics, in turn, are known for their effect on disruption of glucose homeostasis, and depression of respi- ratory and cardiovascular systems. Here, we compared pen- tobarbitone and isoﬂurane for their effects on blood glucose levels. Pentobarbitone did not affect the blood glucose lev- els, but isoﬂurane consistently induced hyperglycemia (Fig. 5). Similar results are widely reported.14,30–33
In a sim- ilar study, Koschwanez et al. tested the effect of isoﬂurane and pentobarbitone on blood glucose levels, and used pen- tobarbitone since it did not cause hyperglycemia for sensor functional efﬁcacy testing.14
They administered a single IP dose of 0.3 mL of 50 mg/mL pentobarbitone (Nembutal Sodium Solution). However, we observed repeated dosing with lower volume of pentobarbitone to be safer at main- taining anesthesia, because the margin between anesthetic and lethal doses for pentobarbitone is very narrow.34
How- ever, concerns are raised because of the low pH of the pen- tobarbitone solution.35
Due to pain that may be caused by the low pH, use of pentobarbitone as an anesthetic is gener- ally discouraged unless it was for nonrecovery procedures.
Similarly, the use isoﬂurane as an anesthetic for glucose tol- erance test is discounted since it offsets the glycemic proﬁle.
Despite the offset, we noticed the glycemic proﬁle was com- parable to that observed with pentobarbitone [Fig. 5(b,c)].
However, it was also shown that the effect of hyperglycemia induced by isoﬂurane can be minimized using analgesia.32,33
We used buprenorphine hydrochloride and carprofen as analgesics to obtain baseline blood glucose levels of 6.526
0.28 and 4.456
0.1 mM/L for isoﬂurane and pento- barbitone, respectively.
Upon IP injection of glucose (1 g/kg), blood glucose levels rose rapidly, peaked at 8.876
0.45 mM/L and
0.53 mM/L, respectively, for pentobarbitone and isoﬂurane and tailed off slowly [Fig. 5(a)]. For isoﬂurane, it took longer for glucose levels to peak and longer to decrease. The difference can be attributed to the continuous dose of isoﬂurane for maintaining anesthesia. Despite the baseline increase of blood glucose levels with the use of iso- ﬂurane, the dynamics of blood glucose levels as measured by the implanted sensor response current was similar to that measured using the commercial blood glucometer [Fig.
5(c)], which dynamic change in blood glucose levels was also similar to that observed with pentobarbitone [Fig.
5(b)]. Thus, with appropriate analgesia, isoﬂurane can serve as an anesthetic for glucose tolerance tests in healthy rats.
Effect of electrospun coatings on the function of glucose biosensors implanted in the subcutaneous tissue of rats.
The sensor conﬁgurations Pt-GOD-8PU-12PU, Pt-GOD- EPU-12PU, Pt-GOD-EPU-6PU10GE, and Pt-GOD-EPU were tested for functional efﬁcacyin vivo
at 1, 3 and 9 weeks after implantation for each implanted sensor. Examples of typical sensor response current curves measuring glucose levels in interstitial ﬂuid as a function of time along with the corresponding change in blood glucose levels are shown in Figure 5(b,c). The sensor response delay was calculated in relation to changes of glucose level in blood as indicated in Figure 5(b,c).
Premature sensor failure is quite common in implant- able glucose monitoring. In this study, 4, 5, 2, and 3 out of 6 sensors were functional at the end of the study period of 9 weeks for Pt-GOD-EPU, Pt-GOD-8PU-12PU, Pt-GOD-EPU- 12PU, and Pt-GOD-EPU-6PU10GE sensors, respectively. 2 and 1 sensors failed by 3 weeks for Pt-GOD-EPU and Pt- GOD-8PU-12PU, respectively. On the other hand, 2 of the 4, and 2 of the 3 nonfunctional sensors in the case of Pt-GOD- EPU-12PU and Pt-GOD-EPU-6PU10GE, respectively, could
and (c) H&E and (d) MT stained section at 9 weeks after implantation, where NF is the native fibrous tissue structure, and I the implant.
not be tested due to broken sensor leads. Of the four func- tional Pt-GOD-EPU-12PU sensors implanted in the rat sub- cutaneous tissue, two failed by 9 weeks, and of the four functional Pt-GOD-EPU-6PU10GE sensors, one failed by 3 weeks. Essentially, at least 50% of the sensors were func- tional till the end of the 9-week study period, which can be
attributed to the larger quantity of glucose oxidase immobi- lized on the cotton-reinforced coil of the working electrode design tested in this study (Fig. 1). Similar correlation of higher levels of GOD loading leading to longerin vivo
sens- ing life was reported earlier.6
Sensor response delay.
The time taken for the implanted glucose biosensors to respond to the high dose of glucose injected in the peritoneum was compared with that in blood and results presented in Figure 6(a). At week 1 after
FIGURE 5. Change in blood glucose concentration: (a) measured using Freestyle Lite blood glucose meter showing the effect of two types of anesthesia on blood glucose levels, (b, c) The typical sensor response current vs. time plot of an implanted sensor and the corre- sponding change in blood glucose levels measured using a commer- cial blood glucose monitor for rats. The anesthesia used for the rats in b and c were sodium pentobarbitone (n516) and isoflurane (n517), respectively. The blue arrow indicates time of injection of a high dose of glucose in the peritoneum. The sensor response delay for the coil-type glucose biosensor implanted in subcutaneous tissue compared to the corresponding change in blood glucose level is indi- cated by the double end arrow (b, c).
FIGURE 6.In vivosensor performance: (a) delay in response to sens- ing glucose in interstitial fluid for coil-type glucose biosensors implanted in the subcutaneous tissue in relation change in blood glu- cose levels as a function of sensor coating configurations; (b) change in sensitivity of glucose biosensors implanted in the subcutaneous tis- sue of rats; and (c) change in sensitivity of glucose biosensors implanted in the subcutaneous tissue of rats normalized to their pre- implantation sensitivities.
response to glucose (<10 min), followed by Pt-GOD-EPU- 6PU10GE and then Pt-GOD-EPU-12PU. The control sensor Pt-GOD-EPU showed the slowest response time of15 min.
By 3 weeks of implantation, Pt-GOD-EPU sensors showed the fastest response time, while that for other sensors with electrospun coatings increased. The trend at week 9 was comparable with that at week 3, except that the sensor Pt- GOD-EPU-6PU10GE showed a decrease in sensor response time. This decrease resulted in its sensor response time to be on par with that of the control sensor Pt-GOD-EPU. The changes in response times could be indicative of the nature of changes in composition of tissue at the sensor tissue interface. The high pore-volume of the electrospun mem- branes at week 1 could be responsible for their better per- meability to glucose and hence faster response time.11
However, at week 3, the tissue build-up at their surface could be responsible for the increase in sensor response delay time. In contrast, the control Pt-GOD-EPU sensor showed initial slower response to glucose which could be due to poor wetting of its EPU membrane, compared to the ﬂuid ﬁlled pores of electrospun membranes. The wetting could have improved with deposition of snugly ﬁt host tis- sue on the EPU membrane, thus lowering the sensor response time thereafter. The sensor response time for Pt- GOD-EPU-6PU10GE decreasing to the level observed with Pt-GOD-EPU control sensor could be due to the resorption of Ge-shell and replacement with collagenous connective tis- sue similar to that observed with PU ﬁlms.
Sensitivity of implanted biosensor to glucose.
The preim- plantationin vitro
sensitivity was 46.136
2.40 nA/mM, respectively, for Pt-GOD- 8PU-12PU, Pt-GOD-EPU, Pt-GOD-EPU-12PU, and Pt-GOD-EPU- 6PU10GE [Fig. 6(b)], which sensitivities are signiﬁcantly higher than the 3.5646
0.054 nA/mM reported by Koschwa- nez et al. for Medtronic MiniMed SOF-SENSORTM
glucose sen- sors.14
The higher sensitivities for our sensors can be attributed to larger quantity of GOD loaded on the working electrodes. Furthermore, among the sensors tested in this study, replacing the traditional solvent cast EPU with electro- spun 8PU as the mass-transport limiting membrane more than doubled thein vitro
sensitivity. Earlier, when we tested 8PU as the mass transport limiting membrane, the sensitivity increased by about 30% compared to that without a mass transport limiting membrane (Pt-GOD).10
In contrast, the cor- responding change for the traditional EPU mass transport limiting membrane was about 10% decrease. This difference manifested as more than double the sensitivity for Pt-GOD- 8PU-12PU compared to Pt-GOD-EPU in this study. This can be attributed to an ordered and gradient transmembrane poros- ity across the 8PU-12PU electrospun coatings on the Pt-GOD sensor surface.
As expected, the sensitivity for all sensor conﬁgurations decreased with increasing implantation time [Fig. 6(b)]. But, it was interesting to note that the higher the preimplanta- tion sensitivity the higher was the sensitivityin vivo, as
observed with Pt-GOD-8PU-12PU sensors. Larger the meas- ured sensor response currents, the lesser will be the signal-
different sensors were normalized to their corresponding preimplantation sensitivities, the percent decrease in sensi- tivity was similar for all sensors. This proportional decrease in sensor sensitivities with time is indicative of the deactiva- tion of the immobilized GOD on the sensor’s working elec- trodes as reported by Valdes and Moussy,6
which is further reiterated by our result that>50% of the implanted sensors
were functional at 9 weeks after implantation. Koschwanez et al. showed that majority of the Medtronic MiniMed SOF- SENSORTM
glucose sensors (with lower preimplantation sen- sitivities compared to sensors tested in our study) failed to respond to the glucose bolus within 2 weeks and all sensors failed by 3 weeks.14
When bioactive 6PU10GE coaxial ﬁber membranes were used as the tissue engineering coatings on the traditional Pt-GOD-EPU sensors, the percent decrease in sensitivity was slowestin vivo
when compared to the rest of the sensors both at 1 and 3 weeks after implantation [Fig. 6(c)], which can be credited to the prevention of dense ﬁbrous capsule on 6PU10GE surface. However, at 9 weeks the advantage of 6PU10GE coatings was lost due to resorption of GE and replacement with collagen, resulting in sensitivities similar to the traditional Pt-GOD-EPU sensors.
Fibro-porous structure of electrospun membranes with average pore sizes of1mm did not inﬂuence the nature of
tissue responses compared to nonporous solvent-cast PU ﬁlm. However, the bioactive 6PU10GE coaxial ﬁber mem- branes, also having similar pore size (1.5mm), allowed
host cell inﬁltration into its ﬁbro-porous bulk. As mass transport limiting membranes, electrospun 8PU membranes showed higher preimplantationin vitro
sensitivity, which translated to higherin vivo
sensitivity. Furthermore, the bio- mimetic 6PU10GE coating prevented ﬁbrous capsule forma- tion on sensor surface, thus increasing sensor sensitivity for at least 3 weeks. To conclude, electrospun membranes can replace traditional mass-transport limiting membranes as well as function as tissue engineering outer coatings to reli- ably prolong thein vivo
sensing lifetime of implantable glu- cose biosensors.
Ning Wang acknowledges the studentship for her Ph.D. from Brunel Institute for Bioengineering, Brunel University. The authors also acknowledge the support and the guidance from Prof. Francis Moussy for this study.
CONFLICT OF INTEREST
No beneﬁt of any kind will be received either directly or indirectly by the author(s).
1. Helton KL, Ratner BD, Wisniewski NA. Biomechanics of the sensor-tissue interface – effects of motion, pressure, and design on sensor performance and the foreign body response – part i:
Theoretical framework. J Diabetes Sci Technol 2011;5:632–646.
2. Wisniewski N, Klitzman B, Miller B, Reichert WM. Decreased ana- lyte transport through implanted membranes: Differentiation of biofouling from tissue effects. J Biomed Mater Res 2001;57:513–
3. Wisniewski N, Moussy F, Reichert WM. Characterization of implantable biosensor membrane biofouling. Fresenius J Anal Chem 2000;366:611–621.
4. Wisniewski N, Reichert M. Methods for reducing biosensor mem- brane biofouling. Colloids Surf B Biointerfaces 2000;18:197–219.
5. Brauker JH, Carr-Brendel V, Tapsak MA. Porous membranes for use with implantable devices. US Patent 8118877; 2012.
6. Valdes TI, Moussy F. In vitro and in vivo degradation of glucose oxidase enzyme used for an implantable glucose biosensor. Dia- betes Technol Ther 2000;2:367–376.
7. Yu B, Moussy Y, Moussy F. Coil-type implantable glucose biosen- sor with excess enzyme loading. Front Biosci 2005;10:512–520.
8. Yu B, Ju Y, West L, Moussy Y, Moussy F. An investigation of long-term performance of minimally invasive glucose biosensors.
Diabetes Technol Ther 2007;9:265–275.
9. Yu B, Moussy Y, Moussy F. Lifetime improvement of glucose bio- sensor by epoxy-enhanced PVC membrane. Electroanal 2005;17:
10. Wang N, Burugapalli K, Song W, Halls J, Moussy F, Ray A, Zheng Y. Electrospun fibro-porous polyurethane coatings for implant- able glucose biosensors. Biomaterials 2013;34:888–901.
11. Wang N, Burugapalli K, Song W, Halls J, Moussy F, Zheng Y, Ma Y, Wu Z, Li K. Tailored fibro-porous structure of electrospun poly- urethane membranes, their size-dependent properties and trans- membrane glucose diffusion. J Memb Sci 2013;427:207–217.
12. Wang N, Burugapalli K, Wijesuriya S, Far MY, Song W, Moussy F, Zheng Y, Ma Y, Wu Z, Li K. Electrospun polyurethane-core and gelatin-shell coaxial fibre coatings for miniature implantable bio- sensors. Biofabrication 2013;6:015002.
13. Reddy SM, Vagama PM. Surfactant-modified poly(vinyl chloride) membranes as biocompatible interfaces for amperometric enzyme electrodes. Anal Chim Acta 1997;350:77–89.
14. Koschwanez HE, Yap FY, Klitzman B, Reichert WM. In vitro and in vivo characterization of porous poly-L-lactic acid coatings for sub- cutaneously implanted glucose sensors. J Biomed Mater Res 2008;87A:792–807.
15. Lee JH, Kopecek J, Andrade JD. Protein-resistant surfaces pre- pared by PEO-containing block copolymer surfactants. J Biomed Mater Res 1989;23:351–368.
16. Sharkawy AA, Klitzman B, Truskey GA, Reichert WM. Engineering the tissue which encapsulates subcutaneous implants. I. Diffusion properties. J Biomed Mater Res 1997;37:401–412.
17. Sharkawy AA, Klitzman B, Truskey GA, Reichert WM. Engineering the tissue which encapsulates subcutaneous implants. II. Plasma- tissue exchange properties. J Biomed Mater Res 1998;40:586–597.
18. Sharkawy AA, Klitzman B, Truskey GA, Reichert WM. Engineering the tissue which encapsulates subcutaneous implants. III. Effec- tive tissue response times. J Biomed Mater Res 1998;40:598–605.
19. Brauker JH, Carr-Brendel VE, Martinson LA, Crudele J, Johnston WD, Johnson RC. Neovascularization of synthetic membranes directed by membrane microarchitecture. J Biomed Mater Res 1995;29:1517–1524.
20. Ju YM, Yu B, Koob TJ, Moussy Y, Moussy F. A novel porous col- lagen scaffold around an implantable biosensor for improving
biocompatibility. I. In vitro/in vivo stability of the scaffold and in vitro sensitivity of the glucose sensor with scaffold. J Biomed Mater Res 2008;87A:136–146.
21. Ju YM, Yu B, West L, Moussy Y, Moussy F. A novel porous collagen scaffold around an implantable biosensor for improving biocom- patibility. II. Long-term in vitro/in vivo sensitivity characteristics of sensors with NDGA- or GA-crosslinked collagen scaffolds.
J Biomed Mater Res 2010;92:650–658.
22. Sanders JE, Cassisi DV, Neumann T, Golledge SL, Zachariah SG, Ratner BD, Bale SD. Relative influence of polymer fiber diameter and surface charge on fibrous capsule thickness and vessel den- sity for single-fiber implants. J Biomed Mater Res 2003;65A:462–
23. Trzebinski J, Moniz AR-B, Sharma S, Burugapalli K, Moussy F, Cass AEG. Hydrogel membrane improves batch-to-batch reprodu- cibility of an enzymatic glucose biosensor. Electroanalysis 2011;
24. Khorshidi S, Solouk A, Mirzadeh H, Mazinani S, Lagaron JM, Sharifi S, Ramakrishna S. A review of key challenges of electro- spun scaffolds for tissue-engineering applications. J Tissue Eng Regen Med 2016;10:715–738.
25. Iatridis JC, Wu J, Yandow JA, Langevin HM. Subcutaneous tissue mechanical behavior is linear and viscoelastic under uniaxial ten- sion. Connective Tissue Res 2003;44:208–217.
26. Burugapalli K, Pandit A. Characterization of tissue response and in vivo degradation of cholecyst-derived extracellular matrix. Bio- macromolecules 2007;8:3439–3451.
27. Bhardwaj N, Kundu SC. Electrospinning: A fascinating fiber fabri- cation technique. Biotechnol Adv 2010;28:325–347.
28. Eichhorn SJ, Sampson WW. Statistical geometry of pores and statistics of porous nanofibrous assemblies. J R Soc Interface 2005;2:309–318.
29. Zhang Y, Ouyang H, Lim CT, Ramakrishna S, Huang Z-M. Electro- spinning of gelatin fibers and gelatin/PCL composite fibrous scaf- folds. J Biomed Mater Res 2005;72B:156–165.
30. Zuurbier CJ, Keijzers PJM, Koeman A, Van Wezel HB, Hollmann MW. Anesthesia’s effects on plasma glucose and insulin and car- diac hexokinase at similar hemodynamics and without major sur- gical stress in fed rats. Anesth Analg 2008;106:135–142.
31. Tanaka K, Kawano T, Tomino T, Kawano H, Okada T, Oshita S, Takahashi A, Nakaya Y. Mechanisms of impaired glucose toler- ance and insulin secretion during isoflurane anesthesia. Anesthe- siology 2009;111:1044–1051.
32. Behdad S, Mortazavizadeh A, Ayatollahi V, Khadiv Z, Khalilzadeh S. The effects of propofol and isoflurane on blood glucose during abdominal hysterectomy in diabetic patients. Diabetes Metab J 2014;38:311–316.
33. Schricker T, Galeone M, Wykes L, Carli F. Effect of desflurane/
remifentanil anaesthesia on glucose metabolism during surgery:
a comparison with desflurane/epidural anaesthesia. Acta Anaes- thesiol Scand 2004;48:169–173.
34. Flecknell PA. Chapter 6—Anaesthesia of common laboratory spe- cies: special considerations. Laboratory Animal Anaesthesia, 3rd ed. San Diego: Academic Press; 2009. p 181241.
35. Svendsen O, Kok L, Lauritzen~a B. Nociception after intraperitoneal injection of a sodium pentobarbitone formulation with and with- out lidocaine in rats quantified by expression of neuronal c-fos in the spinal cord—A preliminary study. Lab Anim 2007;41:197–203.